Transcript of "International Journal of Computational Engineering Research(IJCER)"
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 Prediction of Weld Width of Shielded Metal Arc Weld under Magnetic Field using Artificial Neural Networks R.P. Singh1, R.C. Gupta 2 and S.C. Sarkar 3 1 Mechanical Engineering Depart ment, I.E.T., G.L.A. University Mathura, (U.P.) 2 Mechanical Engineering Depart ment, I.E.T., Lucknow, (U.P) 3 Mechanical Engineering Depart ment, Ku maon Eng ineering College, Dwarahat, (Uttarakhand) I. Abstract: The prediction of the optimal weld bead width is an important aspect in shielded metal arc welding (SMAW) processas it is related to the strength of the weld. This paper focuses on investigation of the development of the simp le and accuratemodel for prediction of weld bead width of butt joint of SMAW process. Artificial neural networks technique was used to traina program in C++ with the help of sufficient number of weld ing data sets having input variables current, voltage, speed ofweld ing and external magnetic field and output variable weld bead width. These variables were obtained after welding mildsteel plates using SMAW process. The welding set-up was mounted on a lathe machine. In this paper, the effect of alongitudinal magnetic field generated by bar magnets on the weld bead width was experimentally investigated. Using theexperimental data a mu lti-layer feed forwa rd art ificial neural network with back propagation algorithm was modeled to pred ictthe effects of weld ing input process parameters on weld width accurately. It was found that welding voltage, arc current,weld ing speed and external magnetic field have the large significant effects on weld bead width. It has been realized that withthe use of the properly trained program, the pred iction of optimal weld bead width becomes much simpler to even a noviceuser who has no prior knowledge of the SMAW process and optimizat ion techniques.Keywords: Artificial Neural Network, Back Propagation, External Magnetic Field, Hidden Layer, Input Process Parameters,Shielded Metal A rc Welding, Weld Bead Width. II. Introduction: Welding is a process of joining different materials. It is mo re economical and is a much faster process compared toboth casting and riveting . The weld bead width is the maximu m width of the weld metal deposited. It influences the fluxconsumption rate and chemistry of the weld metal and hence determines the mechanical properties of the weld . SMAWinput process parameters like welding current, welding speed; open circuit voltage and external magnetic field are h ighlyinfluencing the quality of weld jo ints. The applications of magnetic field in weldin g processes have drawn much attention ofresearchers . Ho wever, the effect of external magnetic field on quality of weld is still lack of understanding. Selection ofprocess parameters has great influence on the quality of a welded connection. A precise means of selection of the processvariables and control of weld bead shape has become essential because mechanical strength of weld is influenced not only bythe composition of the metal, but also by the weld bead shape. The weld bead width is an importan t factor of the shape of theweld. The weld quality can be achieved by meeting quality requirements such as bead geometry which is highly influenced byvarious process parameters involved in the process. Inadequate weld bead dimensions will contribute to failu re of the weldedstructure . A mong all the welding processes, SMAW is very important. The advantages of this method are that it is thesimp lest of the all arc welding processes. The equipment is often small in size and can be easily shifted from one place to theother. Cost of the equipment is very less. This process finds a number of applications because of the availability of a widevariety of electrodes which makes it possible to weld a nu mber of metals and their alloys. The welding of the jo ints may becarried out in any position with highest weld quality and therefore the joints which are difficult to be welded because of th eirposition by automatic welding machines can be easily welded by shielded metal arc welding. Both alternating and directcurrent power sources could be used effectively. Power sources for this type of welding could be plugged into domestic singlephase electric supply, which makes it popular with fabrications of smaller sizes . However, non equilibriu m heating andcooling of the weld pool can produce micro-structural changes which may greatly affect mechanical properties of weld metal.To get the desired weld quality in SMAW process, it is essential to know interrelationships between process parameters andbead geometry as a welding quality. Many efforts have been done to develop the analytical and numerical models to studythese relationships, but it was not an easy task because there were some unknown, nonlinear process parameters. For thisreason, it is good for solving this problem by the experimental models. One of the experimental models is artificial neuralnetworks technique that can be utilized to establish the empirical models for various arc weld ing processes . Investigation intothe relationship between the welding process parameters and bead geometry began in the mid 1900 ’s and regression analysiswas applied to welding geometry research . Many efforts have been carried out for the development of various algorithmsIssn 2250-3005(online) January|| 2013 Page 58
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1in the modeling of arc weld ing process. In the early days, arc welding was carried out manually and the weld quality wastotally controlled by the welder ability. Mc Glone and Chadwick have reported a mathematical analysis correlating processvariables and bead geometry for the submerged arc welding of square edge close butts. Chandel first applied this technique tothe GMA weld ing process and investigated relationship between process variables and bead geometry . These resultsshowed that arc current has the greatest influence on bead geometry, and that mathematical models derived from experimentalresults can be used to predict bead width accurately. Nearly 90% of welding in world is carried out by one or the other arcweld ing process; therefore it is imperat ive to discuss the effects of welding parameters on the weldability of the materialsduring the arc welding. Mild steel was selected for work-p ieces to be welded because it is the most common form of steel asits price is relat ively low while it provides material properties which are acceptable for many applications. III. Experi ment WorkTo investigate the weldment characteristics weld beads were obtained by welding two mild steel flat plates of 150 mm x 50 mm x 5mm dimensions in butt position using mild steel electrodes of 3.15 mm diameter. A manual welding machine was used to weld theplates. A lathe machine was used to provide uniform speed of welding, to support electrode holder and bar magnet. The work piecewas kept on cross slide with some arrangement. Work-piece moves with cross slide. Bar magnet was connected with tailstock with awooden structure Since the weldment characteristics depend on welding current, welding voltage, speed of welding and magneticfield, we select different set of values of these inputs . Welding currents were chosen as 90, 95,100, 105 and 110 A, arc voltageswere chosen as 20, 21, 22,23 and 24V, the welding speeds were chosen as 40, 60 and 80 mm/min and external magnetic fieldstrengths were used as 0, 20,40, 60 and 80 Gauss for the experiments. Current was measured with a clamp meter, voltage wasmeasured with a multi meter and magnetic field was measured with a Gauss meter. To study the bead geometry, each bead wassectioned transversely at two points one near the start (leaving 2 cm from the start) and the other near the end (leaving 2 cm from theend). To get the microstructure, these sectioned beads were ground with emery belt grinder having 0, 2, 3 grade emery papers thenpolished with a double disk polishing machine. Etching was done with a mixture of 2% nitric acid and 98% ethyl alcohol solution.To measure the bead height and bead width of each sample a digital slide caliper was used. The average values of bead height, beadwidth and depth of penetration were measured. Eighteen sets of values out of twenty five such sets obtained were used for training anetwork based on back propagation algorithm. Remaining seven sets of the values were used for prediction. These data sets areshown in table-1. A program of back propagation neural network in C++ was used for training and prediction . In this programone input layer having four neurons, two hidden layers , both having five neurons and one output layer having three neurons, wereused. Table 1 Data for training and prediction Serial Number Current (A) Voltage (V) Welding S peed (mm/min) Magnetic Field (Gauss) Weld idth(mm) Data for 1 90 24 40 0 6.95 Training 2 90 24 40 20 6.94 3 90 24 40 40 6.96 4 90 24 40 60 6.99 5 90 24 40 80 7.03 6 95 20 60 60 6.01 7 95 21 60 60 6.08 8 95 22 60 60 6.10 9 95 23 60 60 6.15 10 95 24 60 60 6.25 11 100 22 40 40 5.94 12 100 22 60 40 5.90 13 100 22 80 40 5.86 14 90 20 80 20 5.91 15 95 20 80 20 5.92 16 100 20 80 20 5.94 17 105 20 80 20 5.95 18 110 20 80 20 5.97 Data for 1 90 23 40 0 6.92Prediction 2 95 22 60 40 6.05 3 95 21 80 60 6.04 4 100 24 40 40 6.99 5 105 21 60 40 5.98 6 105 22 60 20 5.96 7 110 21 60 20 5.97Issn 2250-3005(online) January|| 2013 Page 59
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 Table 2 Measured and predicted values with percentage error S.N. Current Voltage (V) Weldi ng Magnetic Weld Weld Error in (A) Speed Fiel d Width Width Weld (mm/mi n) (Gauss) (mm) (mm) Width Measured % age Predicted 1 90 23 40 0 6.92 6.54 -5.49 2 95 22 60 40 6.05 6.42 +6.12 3 95 21 80 60 6.04 6.44 +6.62 4 100 24 40 40 6.99 6.58 -5.87 5 105 21 60 40 5.98 6.41 +7.20 6 105 22 60 20 5.96 6.40 +7.38 7 110 21 60 20 5.97 6.39 +7.04 Figure 1 Real experimental set-up on a lathe machine1. Mu lti-meter 2. Battery Eliminator 3. Electric Board 4. Gauss Meter 5. Table,6. Measuring Prob 7. Transformer Welding Set 8. Clamp meter 9. Tail Stock 10. Sleeve11. Link (Wood) 12. So lenoid 13. Tool post 14. Iron sheet 15. Workpiece16. Electrode 17. Electrode Holder 18. Metal Strip Connected with head stock19. Head stock 20. Connecting Wires Figure 2 Experimental set-up (Line Diagram)Issn 2250-3005(online) January|| 2013 Page 60
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 IV. Methodol ogy of Artificial Neural Network Modeling Most of the industrial processes are non-linear, co mplex and mo re input variables are involving in processes. Themathematical models are not giving closer approach to describe the behavior of the processes. ANNs are easy to understand,cost effective and have the capability to learn fro m examp les and have found in many industrial application. A NN model hasbeen developed for general applicat ion consisting of the following steps: (i) Database collection, (ii) pre-processing ofinput/output data, (iii) design and training of neural network, (iv) testing of trained network, (v) post processing and (vi) usetrained network for predict ion . The arrangement of neurons into layer and the connection pattern within and between thelayers are called as network architecture. The architecture is consisted of three parts: (i) Input layer receives the weldingparameters, (ii) Hidden layers considered as black boxes and (iii) Output layer obtaining the values of bead geometry. Theperformance of the neural networks depends upon, the n umber of hidden layers and number of neurons in the hidden layers.Hence, optimu m structure is obtained by changing number of hidden layers and neurons by making many attempts. Theappropriate neural networks structure was chosen by the trial and error method. Feed fo rward artificial neural networkstructure was established by keeping four neurons in the input layer, two hidden layers having five neurons in each and oneneurons in output layer using C++. It was trained with help o f back propagation (BP) algorith m. BP is essentially stochasticapproximation to nonlinear regression. Several researchers were used BP to model weld ing processes and predict weldingparameters using Neural network. The designed neural networks structure was 4-5-5-1 (3 neurons in input layer, 5 neurons inboth hidden layers and 1 neuron in output layer). Proposed feed forward neural network arch itecture is shown in figure-3.Non-linearity and input-output mapping are the useful co mplement in neural networks. Hence, it has been adapted to modelthe input-output relation of non-linearity and interconnected system. I/P Hidden Hidden O/P Layer Layer Layer Layer Current Voltage Weld Width Travel speed Magnetic field Figure 3 Feed-forward neural netwo rk (4-5-5-1) architectureIssn 2250-3005(online) January|| 2013 Page 61
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 V. Results and Discussion Table-2 depicted, the measured weld bead width, fro m the experiment and predicted output values us ing artificialneural feed forward network. The measured and predicted output values are close to each other. The aim of this paper showsthe possibility of the use of neural network to predict the weld width accurately. Weld Wi dth The weld width of the welded joints was almost unaffected if the magnetic field was changed from 0 to 20 gauss orfro m 20 to 40 gauss. If the field was increased fro m 40 gauss to 60 gauss, the weld width increased fro m 6.97 mm to 6.99 mm.and if it was increased fro m 60 gauss to 80 gauss, the weld width increased fro m 6.99 mm to 7.03 mm. If the speed of weldingwas increased from 40 mm/ min to 60 mm/ min, the weld width decreased from 5.94 mm to 5.90 mm, and if it was increasedfro m 60 mm/ min to 80 mm/ min, the weld width of the weld decreased from 5.90 mm to 5.86 mm. The effect of voltage waspositive for weld width i.e. if voltage was increased from 20 V to 24 V, the weld width increased from 6.01 mm to 6.25 mm.The increment in current increased the weld width for all the investigated values. If the current was increased fro m 90 A to110 A the weld width increased from 5.91 mm to 5.97 mm. The variat ion of weld width with magnetic field, voltage, weldingspeed and current were shown in figures 4, 5, 6 and 7 respectively. Predicti on of Wel d Wi dth using Artificial Neural NetworksThe developed neural network architecture was trained with help of back propagation algorithm using 18 data sets. Thedeveloped network was tested out of 7 datasets . The training data sets and testing data sets are shown in table-1. The testingdata were not used for training the network. The % age error was calculated between the experimental and predicted values asshown in figure-2. The %age error is ranging between -5.87 to 7.38. The other pred ictions are in between the above ranges andhence are very close to the practical values, which indicate the super predicting capacity of the a rtificial neural network model.Issn 2250-3005(online) January|| 2013 Page 62
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 VI. Discussion In this investigation, an attempt was made to ﬁnd out the best set of values of current, voltage, speed of welding andexternal magnetic field to produce the best quality of weld in respect of weld width . Sh ielded metal arc welding is auniversally used process for joining several metals. Generally in this process speed of welding and feed rate of electrode bothare controlled manually but in the present work the speed of welding was controlled with the help of cross slide of a lathemach ine hence only feed rate of electrode was controlled manually which ensures better weld quality. In the present workexternal magnetic field was utilized to distribute the electrode metal and heat produced to larger area of weld which imp rove sseveral mechanical properties of the weld. The welding process is a very complicated process in which no mathemat icalaccurate relationship among different parameters can be developed. In present work back propagation artificial neuralnetwork was used efficiently in which random weights were assigned to co -relate different parameters which were rect ifiedduring several iterations of training. Finally the improved weights were used for prediction which provided the results verynear to the experimental values. VII. 6. Conclusion The experimental analysis confirms that, artificial neural networks are power tools for analysis and modeling. Resultsrevealed that an artificial neural network is one of the alternatives methods to predict the weld width. Hence it can be proposedfor real time work environ ment. Based on the experimental work and the neural network modeling the following conclusionsare drawn : (1) A strong joint of mild steel is found to be produced in this work by using the SMAW technique.(2) If amperage is increased, weld width generally increases.(3) If voltage of the arc is increased, weld width generally increases.(4) If travel speed is increased weld width generally decreases. (5) If magnetic field is increased weld width, generally increases.(6) Artificial neural networks based approaches can be used su ccessfully for predict ing the output parameters like weld widthof weld as shown in table 2. However the error is rather high as in some cases in predicting weld width it is more than 7percent. Increasing the number of hidden layers and iterat ions can min imize this error.References W.D. Co llister. Material Science and Engineering, An Introduction, John Wiley and Sons, Inc., New Yo rk, USA, 1997. S.V. Nadkarn i. Modern Arc Weld ing Technology, Oxford & IBH Publishing Co. Pvt. Ltd., 1988. M.I. Khan and A.K. Gupta. A study of Hard Facing under Magnetic Field, ASM E Conference, I.I.T. Delh i, 174-176, 1989. W. Robert Messler. Princip les of Welding Processes, Physics, Chemistry and Metallurgy, Wiley, VCH Verlag Gmbh and Co. KgaA Weinheim, 2004. Chien-Yi Lee. A study of an Automatic Welding System, Dissertation of Ph.D., Institute of Mechanical Engineering at National Central University. Jhongli City, Taoyuan County, Taiwan, Republic of China, 2007. Parikshit Dutta and Dilip Ku mar Pratihar. Modeling of TIG Welding Process Using Conventional Regression Analysis and Neural Network Based Approaches, Journal of Materials Processing Technology 184: 56-68, Elsevier, 2007 . R.P. Singh and R.C. Gupta. Application of Art ificial Neural Network to Analy ze and Predict the Mechanical Properties of Shielded Metal Arc Welded Joints under the Influence of External Magnetic Field, International Journal of Engineering Research & Technology (IJERT), Vol. 8, Issue 1, 1-12, , October, 2012. R.P. Singh and R.C. Gupta. Predict ion of Weld Bead Geo metry in Sh ielded Metal A rc Weld ing under External Magnetic Field using Artificial Neural Networks , International Journal of Manufacturing Technology a nd Research, Vo l. 8 number 1, 9-15, 2012. Rajasekaran and G.A. Vijayalakshmi. Neural Networks, Fuzzy Logic and Genetic Algorithms Synthesis and Applications. Prentice Hall of India, 2003. Alvin Ramsey. Assessment of Modeling Abilit ies of Neural Networks, Dissertation, Massachusetts Institute of Technology, 1994.Issn 2250-3005(online) January|| 2013 Page 63
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 Author Rudra pratap Singh received the B.E. degree in Mechanical Engineering fro m MMM EC Go rakhpur in 1992 and the M.Tech. degree in mechanical Engineering in 2009 fro m UPTU Lucknow. During 1992 to 1999 he worked in Jindal Group as a quality control engineer, fro m 1999 to till date he is working in GLA group (now GLA University) Mathura as a faculty in Mechanical Engineering Depart ment. He is pursuing Ph. D. (Registered in, March, 2010) fro m Uttarakhand Technical Un iversity, Dehra dun. He has published seven papers in international journals and three papers in national conferencesIssn 2250-3005(online) January|| 2013 Page 64